Spatial distribution of phases during gradual magnetostructural transitions in copper(ii)-nitroxide based molecular magnets.
Fedin, Matvey V.; Veber, Sergey L.; Bagryanskaya, Elena G.; Romanenko, Galina V.; Ovcharenko, Victor I.; Dalton transactions (Cambridge, England : 2003) 44 (2015) 18823–18830; doi:10.1039/c5dt03441h

data_7036688
_publ_section_title
;
 Spatial distribution of phases during gradual magnetostructural
 transitions in copper(ii)-nitroxide based molecular magnets.
;
_journal_issue                   43
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              18823
_journal_page_last               18830
_journal_paper_doi               10.1039/c5dt03441h
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'C23 H23 Cu F12 N4 O6'
_chemical_formula_weight         742.99
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/6
_audit_update_record
;
2015-08-12 deposited with the CCDC.
2015-09-29 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 125.423(2)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   29.944(2)
_cell_length_b                   9.6596(7)
_cell_length_c                   25.0248(19)
_cell_measurement_reflns_used    9084
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      67.72
_cell_measurement_theta_min      4.34
_cell_volume                     5898.5(7)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0351
_diffrn_reflns_av_unetI/netI     0.0212
_diffrn_reflns_laue_measured_fraction_full 0.989
_diffrn_reflns_laue_measured_fraction_max 0.988
_diffrn_reflns_limit_h_max       35
_diffrn_reflns_limit_h_min       -34
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            81561
_diffrn_reflns_point_group_measured_fraction_full 0.989
_diffrn_reflns_point_group_measured_fraction_max 0.988
_diffrn_reflns_theta_full        67.679
_diffrn_reflns_theta_max         67.713
_diffrn_reflns_theta_min         1.850
_exptl_absorpt_coefficient_mu    2.176
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            dark
_exptl_crystal_density_diffrn    1.673
_exptl_crystal_description       bulk
_exptl_crystal_F_000             2992
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.18
_refine_diff_density_max         0.496
_refine_diff_density_min         -0.358
_refine_diff_density_rms         0.051
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.072
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     940
_refine_ls_number_reflns         10560
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.072
_refine_ls_R_factor_all          0.0333
_refine_ls_R_factor_gt           0.0312
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0462P)^2^+3.2797P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0876
_refine_ls_wR_factor_ref         0.0895
_reflns_Friedel_coverage         0.000
_reflns_number_gt                9820
_reflns_number_total             10560
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5dt03441h2.cif
_cod_data_source_block           100
_cod_depositor_comments
'Adding full bibliography for 7036688--7036694.cif.'
_cod_original_cell_volume        5898.6(8)
_cod_database_code               7036688
_shelxl_version_number           2014/6
_shelx_res_checksum              45974